THE NONLINEAR ABSORPTION OF A STRONG ELECTROMAGNETIC WAVES CAUSED BY CONFINED ELECTRONS IN A CYLINDRICAL QUANTUM WIRE

H. D. Trien and N. V. Nhan

Faculty of Physics, Hanoi University of Science Vietnam National University

334-Nguyen Trai, Thanh Xuan, Hanoi, Vietnam

Abstract—The nonlinear absorption of a strong electromagnetic
wave caused by electrons confined in cylindrical quantum wires
is theoretically studied by using the quantum kinetic equation
for electrons. An analytic expression of the nonlinear absorption
coefficient of a strong electromagnetic wave caused by electrons
confined in a cylindrical quantum wire with a parabolic potential for
electron-optical phonon scattering is obtained. The dependence of the
nonlinear absorption coefficient on the intensity*E*0and the frequency Ω

of the external strong electromagnetic wave, the temperature*T* of the
system and the radius*R*of the wires is strong and nonlinear. Analytic
expression is numerically calculated and discussed for a*GaAs/GaAsAl*

quantum wire. The results are compared with those for normal bulk semiconductors and quantum wells to show the differences.

1. INTRODUCTION

In recent years, the optical properties in bulk semiconductors, as well as low-dimensional systems, have been investigated [1–11]. The linear absorption has been studied in normal bulk semiconductors 1, 2], in two dimensional systems [3–6] and in quantum wires [7, 8]. The nonlinear absorption of a strong electromagnetic wave (EMW) was considered in normal bulk semiconductors [9], quantum wells [10, 16], doping superlattices [17, 18]. Nonlinear optical absorption has also been studied in quantum dots [19]. However, in cylindrical quantum wires, the nonlinear absorption of a strong EMW is still open for studying. In one dimensional systems, the motion of electrons is restricted in two

*Received 9 November 2010, Accepted 4 January 2011, Scheduled 25 January 2011*

dimensions, so they can flow freely in one dimension. The confinement of electrons in these systems changes the electron mobility remarkably. This results in a number of new phenomena, which concern a reduction of the sample dimensions. These effects, for example, electron-phonon interaction and scattering rates [11, 12], the linear and nonlinear optical properties [13, 14], differ from those in bulk semiconductors, as well as two-dimensional systems, and the nonlinear absorption of strong EMW is not an exception. The nonlinear absorption of a strong EMW in a quantum wire will be different from the nonlinear absorption of a strong EMW in bulk semiconductors and two-dimensional. In this paper, we use the quantum kinetic equation for electrons to theoretically study the nonlinear absorption coefficient of a strong EMW by electrons confined in a cylindrical quantum wire (CQW) with a parabolic potential. The problem is considered for electron-optical phonon scattering. Numerical calculations were carried out for specific GaAs/GaAsAl quantum wires.

2. THE NONLINEAR ABSORPTION COEFFICIENT OF A STRONG EMW IN A CQW

We consider a wire of GaAs with a circular cross section with a radius

*R* and a length *Lz* embedded in AlAs. The carriers (electrons) are

assumed to be confined by symmetric parabolic potential of the form

*V* = 1
2*mω*

2

0*r*2*,* (1)

where *m* is the effective mass of electron, and *ω*0 is the effective

frequency of potential well. The total wave function of electrons
in cylindrical coordinates (*r, φ, z*) and the electron energy spectrum
obtained directly from solving Schrodinger equation can be written as

*ψ _{n,`,~}_{p}*(

*r*) =

*√ei~pz*

*Lz*

s
2*n*!
(*n*+*|`|*)!

1

*a*0*e*

*−r*2
2*a*2_{0}

µ

*R*
*a*0

¶* _{|}_{`}_{|}*µ

*r*2
*a*2
0

¶_{|}_{`}_{|}

*L| _{n}`|*

µ

*r*2
*a*2
0

¶

*,* (2)

*ε _{n,`}*(

*~p*) =

*p*2

*z*

2*m* +*ω*0(2*n*+*|`|*+ 1)*,* (3)

where *n* = 0*,* *±*1 *±*2*, . . .* is the azimuthal quantum number, *`* =
1*,* 2*,* 3*, . . .* is the radial quantum number;*~p*= (0*,*0*, pz*) is the electron

wave vector (along the wire’s*z* axis); *L|n`|*(*x*) is a generalized lagrange

polynomial;*a*0= 1*/√mω*0 (in this paper, we select~= 1).

*~*

*E*_{0}sin(Ω*t*), can be written as

*H* = X

*n,l,~p*
*ε _{n,l}*

³

*~p−e*
*cA~*(*t*)

´

*a*+_{n,l,~}_{p}*a _{n,l,~}_{p}*+X

*~*
*q*

*ω b*+_{~}_{q}b_{~}_{q}

+ X

*n,l,n0 _{,`}0_{,~}_{p,~}_{q}*

*C _{~}_{q}I_{n,l,n}0_{,`}0*(

*~q*)

*a*+

*n,l,~p+~q* *an0,`0,~p*

³

*b _{~}_{q}*+

*b*+

_{−}_{~}_{q}´

*,* (4)

where *e* is the electron charge; *c* is the velocity of light; *A~*(*t*) =

*c*

Ω*E~*0cos(Ω*t*) is the vector potential; *E~*0 and Ω are the intensity and

the frequency of the EMW;*a*+* _{n,`,~}_{p}* (

*a*) is the creation (annihilation) operator of an electron;

_{n,`,~}_{p}*b*+

*(*

_{~}_{q}*b*) is the creation (annihilation) operator of a optical phonon for a state having wave vector

_{~}_{q}*~q*;

*ω*is the frequency of a optical phonon; and

*C*is the electron-optical phonon interaction constant, which can be taken as [1, 5, 6]

_{~}_{q}*|C~q|*2 =*e*2*ω*(1*/χ∞−*1*/χ*0)*/*2*²*0*q*2*V*0*,* (5)

where *²*0 is the permittivity of free space; *V*0 is the normalization

volume, and *χ∞*; and *χ*0 are the high-frequency dielectric constants

and low-frequency dielectric constants, respectively. *I _{n,l,´}_{n,}*´

*(*

_{l}*~q*) is the

electron form factor and can be written as

*I _{n,`,n}0*

*`0*(*~q*) =

2

*R*2

Z _{R}

0

*ψn,`*(*r*)*eiqrψ _{n}∗0_{,`}0*(

*r*)

*rdr.*(6)

The carrier current density*~j*(*t*) and the nonlinear absorption coefficient
of a strong electromagnetic wave *α* take the form [9, 10, 15]

*~j*(*t*) = *e*

*m*

X

*n,`,~p*

³

*~p−e*
*cA~*(*t*)

´

*nn,`,~p*(*t*)*,* (7)

*α* = 8*π*

*c√χ∞E*02

D

*~j*(*t*)*E~*_{0}sin Ω*t*

E

*t* (8)

where *nn,`,~p*(*t*) is the electron distribution function; *hXit* means the

usual thermodynamic average of *X* at moment *t*; and *χ∞* is the

high-frequency dielectric constant. In order to establish analytical
expressions for the nonlinear absorption coefficient of a strong EMW
by electrons confined in a CQW, we use the quantum kinetic equation
for particle number operator of an electron*n _{n,`,~}_{p}*(

*t*) =

*ha*+

_{n,`,~}_{p}a_{n,`,~}_{p}i_{t}*i∂nn,`,~p*(*t*)

*∂t* =

Dh

*a*+_{n,`,~}_{p}a_{n,`,~}_{p}, H

iE

*t* (9)

confined in a CQW. Using the first-order tautology approximation
method: *n _{n,`,~}_{p}*(

*t0*

_{)}

_{≈}

_{n}*n,`,~p*, *nn,`,~p+~q*(*t0*) *≈* *nn,`,~p+~q*, *nn,`,~p−~q*(*t0*) *≈*
*n _{n,`,~}_{p}_{−}_{~}_{q}* (This approximation has been applied to a similar exercise
in bulk semiconductors [15] and quantum wells [10]) to solve this
equation, we obtain the expression of electron distribution function,

*n _{n,`,~}_{p}*(

*t*):

*n _{n,`,~}_{p}*(

*t*) =

*−*X

*~*

*q,n0*

_{,`}0*|C _{~}_{q}|*2

*|I*(

_{n,`,n}0_{,`}0*~q*)

*|*2

*∞*

X

*k,l=−∞*

1

*l*Ω*e*

*−ilΩt _{J}*

*k*

Ã

*e ~E*_{0}*~q*
*m*Ω2

!

*×J _{k+l}*

Ã

*e ~E*0*~q*
*m*Ω2

! (

*−* *n*¯*n,`,~p*(*N~q*+ 1)*−n*¯*n0,`0,~p+~qN~q*
*εn0 _{,`}0*(

*~p*+

*~q*)

*−ε*(

_{n,`}*~p*) +

*ω−k*Ω +

*iδ*

*−* *n*¯*n,`,~pN~q−*¯*nn0,`0,~p+~q*(*N~q*+ 1)
*εn0 _{,`}0*(

*~p*+

*~q*)

*−ε*(

_{n,`}*~p*)

*−ω−k*Ω +

*iδ*

+ *n*¯*n0,`0,~p−~q*(*N~q*+ 1)*−*¯*nn,`,~pN~q*

*ε _{n,`}*(

*~p*)

*−ε*(

_{n}0_{,`}0*~p−~q*) +

*ω−k*Ω +

*iδ*

+ *n*¯*n0,`0,~p−~qN~q−n*¯*n,`,~p*(*N~q*+ 1)

*εn,`*(*~p*)*−εn0 _{,`}0*(

*~p−~q*)

*−ω−k*Ω +

*iδ*

)

*,* (10)

where *N _{~}_{q}* (¯

*n*) is the time independent component of the phonon (electron) distribution function;

_{n,`,~}_{p}*Jk*(

*x*) is the Bessel function; and

the quantity *δ* is infinitesimal and appears due to the assumption of
an adiabatic interaction of the electromagnetic wave. We insert the
expression for *n _{n,`,~}_{p}*(

*t*) into the expression for

*~j*(

*t*) and then insert the expression for

*~j*(

*t*) into the expression for

*α*in Eq. (8). Using the properties of Bessel function and realizing the calculations, we obtain the nonlinear absorption coefficient of a strong EMW by confined electrons in a CQW as

*α* = 8*π*3*e*2Ω*kbT*

*c√χ∞E*02*²*0*V*0

µ 1

*χ _{∞}*

*−*

1

*χ*_{0}

¶ X

*n,`,n0,`0*

X

*~*
*q,~p*

*|I _{n,`,n}0_{,`}0*(

*~q*)

*|*2 1

*q*2

*×*

*∞*

X

*k=−∞*

£ ¯

*nn,`,~p−n*¯*n0 _{,`}0_{,~}_{p+~}_{q}*

¤

*kJ _{k}*2

Ã

*e ~E*_{0}*~q*
*m*Ω2

!_{n}

*δ*(*εn0 _{,`}0*(

*~p*+

*~q*)

*−ε _{n,`}*(

*~p*)+

*ω−k*Ω) +

*δ*¡

*ε*(

_{n}0_{,`}0*~p*+

*~q*)

*−ε*(

_{n,`}*~p*)

*−ω−k*Ω

¢ o

*,*(11)

where *V*0 is the normalization volume, and *δ*(*x*) is the Dirac delta

*|k*Ω*−ω| ¿* *ε*¯ must be satisfied [9, 10]. We restrict the problem to
the case of absorbing a photon and consider the electron gas to be
non-degenerate:

¯

*n _{n,`,~}_{p}*=

*n∗*

_{0}exp µ

*−εn,`*(*~p*)
*k _{b}T*

¶

, with*n∗*_{0} = *n*0(*eπ*)

3 2

*V*0(*m*0*kbT*)

3 2

(12)

where *m*0 is the mass of a free electron; *n*0 is the electron density

in a CQW; and *kb* is the Boltzmann constant. Using the Bessel

function and the energy spectrum of an electron in a CQW, we have an explicit formula of the nonlinear absorption coefficient in a CQW with a parabolic potential:

*α*=

*√*

2*πe*4_{n}∗

0(*kbT*)3/2

4*c²*0*√mχ∞*Ω3*V*0

µ
1
*χ∞* *−*
1
*χ*0
¶ X

*n,`,n0 _{,`}0*

*|In,`,n0 _{,`}0*(

*~q*)

*|*2

*×*

( exp

µ

*B*(+*ω*)

*kbT*

¶· exp

µ

*−*Ω+*ω*
*kbT*

¶

*−*1
¸ ·

1+3*e*

2* _{E}*2
0

*kbT*

8*m*Ω4

µ
1+*B*

+_{(}_{ω}_{)}

2*kbT*

¶¸

+exp µ

*B*(*−ω*)

*kbT*

¶· exp

µ

*−*Ω*−ω*
*kbT*

¶

*−*1
¸·

1+3*e*

2* _{E}*2
0

*kbT*

8*m*Ω4

µ

1+*B*(*−ω*)
2*kbT*

¶¸)

*,*(13)

where *B*(*±ω*) = *ω*0(2*n0−*2*n*+*|`0| − |`|*)*±ω−*Ω. From the analytic

expression for the nonlinear absorption coefficient of a strong EMW
caused by confined electrons in CQWs with an parabolic potential
(Eq. (13)), we can see that when the term proportional to the quadratic
intensity of the EMW (*E*2

0) tends toward zero, the nonlinear result will

become a linear result.

3. NUMERICAL RESULTS AND DISCUSSIONS

In order to clarify the results that have been obtained, in this section,
we numerically calculate the nonlinear absorption coefficient of a strong
EMW for a*GaAs/GaAsAl*CQW. The nonlinear absorption coefficient
is considered as a function of the intensity *E*0 and the energy of the

strong EMW, the temperature *T* of the system, and the parameters
of the CQW. The parameters used in the numerical calculations [6, 13]
are *ξ* = 13*.*5 eV, *ρ* = 5*.*32 gcm*−*3_{,} _{υ}

*s* = 5378 ms*−*1, *²*0 = 12*.*5,
*χ∞* = 10*.*9, *χ*0 = 13*.*1, *m* = 0*.*066*m*0, *m*0 being the mass of free

electron, ~*ω* = 36*.*25 meV, *kb* = 1*.*3807*×*10*−*23j/K, *n*0 = 1023m*−*3,
*e*= 1*.*60219*×*10*−*19_{C,} _{~}_{= 1}_{.}_{05459}_{×}_{10}*−*34_{j}_{·}_{s.}

2 4 6 8 10 x 10-8 0 0.2 0.4 0.6 0.8 1 1.2 1.4 1.6

Radius of wire (m)

Nonlinear absorption coefficient (Arb. Units)

T=273(K) T=270(K)

Figure 1. Dependence of *α* on
radius of wire at different values
of temperature *T*.

1 2 3 4 5 6 7 8 9 10

x 10-8

0 0.2 0.4 0.6 0.8 1 1.2 1.4 1.6 1.8 2

Radius of Wire (nm)

Nonlinear absorption coefficient (Arb. Units)

0=10 12 s-1 0=2x10 12 s-1 ω ω

Figure 2. Dependence of *α* on
radius of wire at different values
of *ω*0.

50 100 150 200 250 300

1 1.2 1.4 1.6 1.8 2 2.2 2.4 2.6 2.8 Temperature (K)

Nonlinear absorption coeffici

ent (Arb. Units)

=7x1013_{ s}-1

=6x1013 s-1 Ω Ω

Figure 3. Dependence of*α* on*T*

at different values of Ω.

1 2 3 4 5 6

x 106 0.78 0.79 0.8 0.81 0.82 0.83 0.84

Intensity E0 (V/m)

Nonlinear absorption coefficient

(Arb. Units)

T=270 (K) T=273 (K)

Figure 4. Dependence of *α* on

*E*_{0} at different values of*T*.

that the absorption coefficient depends strongly and nonlinearly on
the radius *R* of wire. The absorption has the same maximum values

(peaks) at *R* *∼* 48 nm. At *T* = 270 and *T* = 273, the maximum

values of absorption coefficient are 1.47 m*−*1 and 1.17 m*−*1 respectively.
The radius *R* of wire at which *α* has a maximum is not changed as
the temperature *T* of the system is varied. However, Figure 2 shows
that the radius *R* of wire at which *α* has a maximum changed if
the effective frequency of potential well *ω*0 is varied. For example,

at *ω*0 = 1012s*−*1 and *ω*0 = 2 *×*1012s*−*1 the peaks correspond to
*R* *∼* 48 nm and *R* *∼* 34 nm, respectively. The nonlinear absorption
coefficient depends strongly on the effective frequency of potential
well *ω*0. At *ω*0 = 1012s*−*1 and *ω*0 = 2 *×*1012s*−*1, the maximum

values of absorption coefficient are 1.47 m*−*1 _{and 1.82 m}*−*1 _{respectively.}

radius at which the nonlinear absorption coefficient has a maximum
value only depends on the structural parameter of wire (the effective
frequency of potential well *ω*_{0}). Figure 3 shows the dependence of
the nonlinear absorption coefficient *α* on the temperature *T* of the
system at different values of frequency Ω of the external strong EMW.
It can be seen from this figure that the nonlinear absorption coefficient

*α* depends strongly and nonlinearly on *T*. The nonlinear absorption
coefficient*α*is increased when the temperature*T* increases. But when

*α* has the maximum value, if the temperature continues to increase,*α*

decreases. This fact was not seen in bulk semiconductors [9] as well as
quantum wells [10]. This can be explained that: At high temperatures,
conditions*εn+1−εnÀkbT* no longer is satisfied. The dependence of
*α* due to the confinement of electrons in one-dimensional systems is
significantly reduced. The temperature*T* of the system at which*α*has
a maximum is changed as frequency Ω of the external strong EMW is
varied. For example, at Ω = 6*×*1013_{s}*−*1_{and Ω = 7}_{×}_{10}13_{s}*−*1 _{the peaks}

correspond to *T* *∼*160 K and 180 K, respectively. Figure 4 shows the
dependence of the nonlinear absorption coefficient *α* on the intensity

*E*0 of EMW at different values of the temperature*T* of the system. It

can be seen from this figure that the nonlinear absorption coefficient
depends strongly and nonlinearly on the intensity *E*0 of EMW. The

nonlinear absorption coefficient *α* increases when the intensity *E*0 of

EMW increases. Figure 5 presents the dependence of *α* on the EMW
energy at different values of the effective frequency of potential well*ω*0.

It is seen that *α* has the same maximum values (peaks). The EMW
energy at which*α*has a maximum is~Ω = 0*.*03625 eV (Ω*≡ω*) and not
changed as the effective frequency of potential well *ω*0 is varied. This

means that *α* depends strongly on the frequency Ω of the EMW, and

0.020 0.04 0.06 0.08 0.1 0.12 0.5

1 1.5 2 2.5 3 3.5

Photon energy (eV)

Nonlinear absorption coefficient (Arb. Units)

0=10 12

s-1

0=1.3x10
12_{ s}-1

ω

ω

resonance conditions are determined by the EMW energy. Maximum
value of *α* varies when changing the effective frequency of potential
well *ω*_{0}. At *ω*_{0} = 1012_{s}*−*1 _{and} _{ω}

0 = 1*.*3*×*1012s*−*1, the maximum

values of absorption coefficient are 1.5 m*−*1 _{and 3.2 m}*−*1 _{respectively.}

In addition, it can be seen from Figures 1–5 that, different from
normal bulk semiconductor [9] and quantum wells [10], the nonlinear
absorption coefficient *α* in quantum wires is bigger. It is explained
that when electrons is confined in a quantum wire, the electron energy
spectrum continues to be quantized. So the absorption of a strong
electromagnetic wave is better. This fact is also reflected in the
expressions of the nonlinear absorption coefficient (Eq. (13)). Besides
the sum over quantum *n* (as in quantum well), the expressions of the
nonlinear absorption coefficient in quantum wire have the sum over the
quantum number *`*.

4. CONCLUSION

In this paper, we have obtained analytical expression for the nonlinear absorption of a strong EMW by confined electrons in CQW for the case electron-optical phonon scattering and numerically calculate for a

*GaAs/GaAsAl* quantum wire. The analytical results and numerical

results obtained for a *GaAs/GaAsAl* CQW show that *α* depends

strongly and nonlinearly on the intensity *E*0 and frequency Ω of the

external strong EMW, the temperature *T* of the system and the
radius *R* of wires. Results also show that the nonlinear absorption
coefficient has maximum values at a value determined by wire’s radius,
at which the nonlinear absorption coefficient has a maximum value only
dependent on the structural parameter of wire (the effective frequency
of potential well *ω*0). In the dependence of *α* on the temperature

T, *α* also has the same maximum value (peaks). From this peak, if
the temperature continues to increase, *α* decreases because at high
temperatures, conditions *ε _{n+1}*

*−*

*ε*

_{n}*À*

*k*no longer are satisfied. The dependence of

_{b}T*α*due to the confinement of electrons in one-dimensional systems is significantly reduced. These new contributions are not seen in other articles [9, 10, 16–19]. The nonlinear absorption coefficient in quantum wire is larger than the nonlinear absorption coefficient in normal bulk semiconductors [9] and two dimensional systems [10, 18]. The results show a geometrical dependence of

*α*due to the confinement of electrons in one dimensional systems. In addition, from the analytic result, we see that when the term in proportion to quadratic the intensity of the EMW (

*E*2

0) (in the expression of the

ACKNOWLEDGMENT

This work is completed with financial support from the Vietnam National Foundation for Science and Technology Development.

REFERENCES

1. Shmelev, G. M., L. A. Chaikovskii, and N. Q. Bau, “HF
conduction in semiconductors superlattices,” *Sov. Phys. Tech.*

*Semicond.*, Vol. 12, 1932, 1978.

2. Matsumoto, Y., S. Ozaki, and S. Adachi, “Optical properties of
the bulk amorphous semiconductor ZnIn2Te4,” *J. Appl. Phys.*,
Vol. 86, 3705, 1999.

3. Brown, E. R. and S. J. Eglash, “Calculation of the intersubband
absorption strength in ellipsoidal-valley quantum wells,” *Phys.*

*Rev. B*, Vol. 41, 7559, 1990.

4. Wu, J.-J., D. Chen, K.-L. Liao, T.-J. Yang, and W.-L. Ouyang,
“The optical properties of Bragg fiber with a fiber core of
2-dimention elliptical-hole photonic crystal structure,” *Progress In*

*Electromagnetics Research Letters*, Vol. 10, 87–95, 2009.

5. Bau, N. Q. and T. C. Phong, “Calculations of the absorption
coefficient of a weak electromagnetic wave by free carriers in
quantum wells by the Kubo-Mori method,” *J. Japan Phys. Soc.*,
Vol. 67, 3875, 1998.

6. Bau, N. Q., N. V. Nhan, and T. C. Phong, “Calculations of the absorption coefficient of a weak electromagnetic wave by free carriers in doped superlattices by using the Kubo-Mori method,”

*J. Korean Phys. Soc.*, Vol. 41, 149, 2002.

7. Ibragimov, G. B., “Optical intersubband transitions in quantum
wires with an applied magnetic field,” *Semiconductor Physics,*

*Quantum Electronics and Optoelectronics*, Vol. 7, 283, 2004.

8. Bau, N. Q., L. Dinh, and T. C. Phong, “Absorption coefficient
of weak electromagnetic waves caused by confined electrons in
quantum wires,” *J. Korean Phys. Soc.*, Vol. 51, 1325, 2007.
9. Pavlovich, V. V. and E. M. Epshtein, “Quantum theory

of absorption of electronmagnetic wave by free carries in
simiconductors,” *Sov. Phys. Solid State*, Vol. 19, 1760, 1977.
10. Bau, N. Q., D. M. Hung, and N. B. Ngoc, “The nonlinear

absorption coefficient of a strong electromagnetic wave caused
by confined electrons in quantum wells,” *J. Korean Phys. Soc.*,
Vol. 54, 765, 2009.

V. V. Mitin, “Electron-optical-phonon scattering rates in a
rectangular semiconductor quantum wire,”*J. Appl. Phys.*, Vol. 70,
319, 1991.

12. Antonyuk, V. B., A. G. Malshukov, M. Larsson, and K. A. Chao,
“Effect of electron-phonon interaction on electron conductance in
one-dimensional systems,”*Phys. Rev. B*, Vol. 69, 155308, 2004.
13. Chernoutsan, K., V. Dneprovskii, S. Gavrilov, V. Gusev,

E. Muljarov, S. Romano, A. Syrnicov, O. Shaligina, and
E. Zhukov, “Linear and nonlinear optical properties of excitons
in semiconductordielectric quantum wires,” *Physica E*, Vol. 15,
111, 2002.

14. Rossi, F. and E. Molinari, “Linear and nonlinear optical properties
of realistic quantum-wire structures: The dominant role of
Coulomb correlation,”*Phys. Rev B*, Vol. 53, 16462, 1996.

15. Malevich, V. L. and E. M. Epstein, “Nonlinear optical properties
of conduction electrons in semiconductors,” *Sov. Quantum*

*Electronic*, Vol. 1, 1468, 1974.

16. Bau, N. Q., L. T. Hung, and N. D. Nam, “The nonlinear
absorption coefficient of a strong electromagnetic wave by confined
electrons in quantum wells under the influences of confined
phonons,” *Journal of Electromagnetic Waves and Applications*,
Vol. 24, No. 13, 1751–1761, 2010.

17. Bau, N. Q., D. M. Hung, and L. T. Hung, “The influences
of confined phonons on the nonlinear absorption coefficient of
a strong electromagnetic wave by confined electrons in doping
superlattices,” *Progress In Electromagnetics Research Letter*,
Vol. 15, 175–185, 2010.

18. Bau, N. Q. and D. M. Hung, “Calculation of the nonlinear
absorption coefficient of a strong electromagnetic wave by confined
electrons in doping superlatices,” *Progress In Electromagnetics*

*Research B*, Vol. 25, 39–52, 2010.